Romjist_FINALROMANIAN JOURNAL OF INFORMATION SCIENCE AND TECHNOLOGY
Volume .., Number .., 2017, 201–217
Fabrication and characterization of suspended microstructures of
C. Pachiu (1), T. Sandu (1,2), C.Tibeica (1,2), L. M. Veca (1), R.
M. Popescu (1), R. Gavrila (1), C. Popov (3), V. Avramescu (1) (1)
National Institute for Research and Development in
Microtechnologies - IMT Bucharest,
126A Erou Iancu Nicolae, Bucharest, Romania
(2) Research Centre for Integrated Systems, Nanotechnologies, and
Carbon Based Materials - IMT Bucharest
(3) Institute of Nanostructure Technologies and
Analytics, University of Kassel, Heinrich-Plett-Strasse 40,
34132 Kassel, Germany
Abstract. The fabrication of various suspended microstructures made
from ultrananocrystalline diamond was performed without sacrificial
layer. Arrays of bridges and cantilevers of various dimensions were
successfully fabricated by a well-controlled process. Mechanical
characterizations and finite element calculations allowed us to
estimate both the Young’s modulus as well as the residual stress
built in the ultrananocrystalline diamond film.
Keywords: residual stress, ultrananocrystalline diamond, MEMS,
1. Introduction and preliminary results
Diamond, in its single-crystal form, possesses rather exceptional
properties [1, 2]
that are attractive for many applications working in extreme
conditions such as
environments with high temperature or/and corrosive chemicals,
switches, etc. Its mechanical properties (hardness of 100 GPa,
Young's modulus of 1200
GPa, very good wear resistance and low friction) together with its
stability and biocompatibility make diamond and diamond-based
electromechanical systems (MEMS) good for environmentally friendly
information technology, automotive and aerospace industries, and
medicine [3, 4].
These impressive properties of single-crystal diamond are expected
to be found
to a large extent into nanocrystalline diamond (NCD) and
(UNCD). NCD and UNCD are two-phase systems composed of
diamond grains and amorphous carbon that fills the
inter-crystalline space. The NCD
films contain grains with sizes between tens of nm and one µm. On
the other hand, the
UNCD films have grains with sizes varying from 2 to 10 nm
Being grown much easier than the single-crystalline films [6, 7]
smooth surfaces, uniform thicknesses, and mechanical properties
close to those of
single-crystal diamond, the UNCD films are ideal for MEMS
applications. . The
fabrication of MEMS devices is a multi-step process of deposition,
patterning, and selective etching of a multi-layered thin film .
In this fabrication
process a sacrificial silicon dioxide layer is used. The
sacrificial layer is deposited/grown
with the scope of supporting the subsequent device layer and later
is removed by a
selective isotropic etching in order to release a free-standing
MEMS device. Thus, the
structure of the multi-layered thin film consists of a device layer
at the top, a sacrificial
layer in the middle which is supported by a substrate at the
bottom. During the final
stages of removing the sacrificial layers stiction problems may
appear. Stiction is the
unintentional adhesion of otherwise freestanding structures to the
substrate. There are
several ways to deal with the stiction problem. One of them is to
roughen the surface to
reduce the contact area . There are also other ways to solve
the problem like the
changing of wetting properties of the solution-substrate interface
, the use of a
supercritical drying , etc.
In this work we follow a different approach by omitting completely
layer to fabricate suspended UNCD microstructures. In other words,
thin film is just a micrometer-sized UNCD film directly deposited
on the silicon
substrate. Then, while maintaining the integrity of the UNCD
remove sufficient material from underneath of the UNCD device by a
etching process to obtain suspended microstructures. The main
motivation for not using
a sacrificial layer is the fact that a direct growth of UNCD films
on SiO2 is not
straightforward and it needs the addition of Ar in plasma for
successful growth of
UNCD film on sacrificial layer SiO2 . Thus, we were able to
structures like bridges and cantilevers without the use of a
sacrificial layer. Moreover, it
is well-known that during the fabrication process, the mechanical
stress, in general, and
the residual stress, in particular, may play an important role for
especially in the final stages of fabrication after the release
from the substrate . We
also evaluated the residual compressive stress of the UNCD film
deposited on the silicon
substrate by measuring the Young's modulus and using its value in
FEM (Finite Element
Method) mechanical simulations. The work has the following
structure: section 2
presents the process fabrication of suspended UNCD based
microstructures; section 3 is
dedicated to the morphological and mechanical characterization and
to discussions; in
the last section 4 we conclude the work.
2. UNCD device fabrication
In this work we used UNCD films grown by microwave plasma
chemical vapor deposition (MW-PECVD) on 3-inch (100) Si wafers .
pattering was obtained first by fabricating an aluminum (Al) mask
directly on the UNCD
film. Then, the UNCD microstructures were obtained with plasma
assisted etching of (a)
the UNCD film in oxygen atmosphere and (b) the silicon substrate in
(SF6) (Reactive Ion Etching - RIE with EtchLab SI 220, Sentech
etching processes were performed in the presence of the metallic
mask. Some of these
results showing released microstructures were presented in a recent
In the following we present the details of the full fabrication
fabrication starts with the deposition of the metal layer. Prior to
metal deposition, the
UNCD surface was treated in a cleaning hot piranha solution (H2SO4,
H2O2 3:1 at
150oC for 5 min, followed by washing in deionized water and drying
in nitrogen) to
modify the surface into oxygen- and hydroxyl-terminated one for a
The metal deposition was made directly on the UNCD film. Different
photoresists, and metals with different etch rates and selectivity
can be used in mixture
of oxygen and sulfur hexafluoride (SF6) RIE, but we have chosen
aluminum as a mask in
UNCD etching process because it has a significantly lower etch rate
and a stronger
resistance to etching than a photoresist [15, 16]. Thus, a 500 nm
thick Al film was
sputtered onto the UNCD layer (AUTO 500, BOC Edwards) (Figure 1.a,
In a second step, the photoresist was deposited by coating to
configure the mask on
Al layer (Figure 1.c). Using the classical photolithography
technique, the metallic mask
was patterned with the designed geometry (Figure 1.d). To obtain
a 1.5 µm thick positive photoresist was used (HPR-504, Fujifilm),
spin-coated at 3000
rpm, followed by the post-baking at 100o C for 30 min, and
developed in 15-30 seconds
with HPRD-437 developer. The mask contained the following
microstructures: arrays of micro-cantilevers and bridges.
The process of metal mask fabrication was continued with the wet
etching of the metal layer through the patterned photoresist (3: 3:
1: 1 H3PO4: HNO3:
CH3COOH: H2O at 40° C for 2 min)  at 40oC for about 2 min,
followed by the
removal of the remaining photoresist.
In this way, we obtained the metallic protective mask that is
needed to fabricate the
UNCD - based microstuctures such as micro-cantilevers and
Figure 1. Fabrication flow of UNCD microstructures: (a) the UNCD
film deposited on Si; (b) the deposition of the metal layer used to
fabricate the protecting mask; (c) the photoresist deposition; (d)
the lithographic process pattering
the metallic layer; (e) the processes of etching the UNCD film and
the Si substrate to release the microstructures.
Using the metallic mask, the UNCD film was processed with selective
reactive ion etching (RIE) in oxygen atmosphere, with 450 Watts RF
power under a
pressure of 15 Pa. The etching rate of the UNCD film was
approximately 65 nm/min
using an O2 gas flow rate of 50 sccm for 10 min.
In order to release the patterned microstructures, the process was
two recipes for isotropic etching of Si substrate (Figure 1.e). The
first etching recipe was
as follows: mixture of oxygen and sulfur hexafluoride (SF6) RIE for
10 min, with an O2
gas flow rate of 50 sccm and SF6 gas flow rate of 10 sccm. The
etching rate was
approximately 90 nm/min. The second etching recipe was performed at
the same RF
power and gas pressure using not more than SF6, with a gas flow
rate of 100 sccm for 10
min. The above patterning processes were successfully tested and
consequently arrays of
bridges and cantilevers were fabricated using them.
3. Results and discussions
Various suspended microstructures were fabricated and inspected by
resolution electron microscopy in order to evaluate the
technological efficiency of the
processes described in the previous section. Detailed examination
of the fabricated
structures was conducted by SEM (Scanning Electron Microscopy),
NanoSEM 630 (former FEI Company, today Thermo Fisher Scientific,
One of the challenges in the fabrication of UNCD suspended
the robustness of Al mask with respect to the etching agents used
in the etching
processes. During the UNCD etching process, oxygen removes also Al
debris that are taken away from the mask and moved into the regions
where the UNCD
film is supposedly etched away. The debris acts as micro-masks for
the UNCD material
in the etching region, hence the UNCD etching is incomplete .
Initially, we thought
that, to get rid of remaining UNCD material, it is better to keep
oxygen as an etching
agent together with SF6 during the Si etching process (the first
recipe described in the
However, it turns out that not removing the photoresist in the
fabricating the Al mask together with the use of SF6 alone as an
etching agent for Si
substrate lead to a successful fabrication of suspended
microstructures (Figure 4).
Figure 2. SEM micrographs of arrays of bridges fabricated from UNCD
films in the oxygen and sulfur hexafluoride mixture RIE process.
Various degrees of buckling indicating a compressive stress can be
observed. In the zoom
images the presence of debris can be seen.
Figure 4. SEM micrographs of cantilevers fabricated from UNCD films
by etching the Si substrate with sulfur hexafluoride only. As it
can be seen in the zoom images the debris effects were minimized.
The images were taken at an intermediate phase of the process, when
the Al mask was not removed from the microstructures. Al from the
creates an additional stress that warps the cantilevers.
From Figures 2 and 3 one can see that the bridges and the
cantilevers are completely
released from substrate. The effect of adding oxygen in the process
of Si etching can be
seen in zoomed images presented in Figures 2 and 3. Nevertheless,
this process creates
debris acting as micro-masks which make a rough and uneven
substrate underneath of
fabricated microstructures. On the contrary, when only SF6 is used
to etch Si, the
substrate underneath of microstructures looks much better, hence
the effect of the debris
is minimized (Figure 4). We notice here that the images shown in
Fig. 4 were taken
before removing the Al mask. The upward bending of cantilevers
indicates an induced
stress by the Al mask.
3.2. Young modulus measurements of UNCD films
The Young's modulus of the UNCD films was measured by
indentation (Nano Indentation) technique employing a G200 Nano
Technologies, former Agilent Technologies). The indenter tip used
in the measurements
was a three-sided pyramidal Berkovich diamond tip.
The patented Continuous Stiffness Measurement (CSMTM) method
employed. It allowed the assessment of the mechanical behavior of
composing the film independently from that of the underlying
substrate. In the CSM
method, an oscillating force considerably smaller than the nominal
load is superimposed
on the quasi-static indentation. The sample response is then
analyzed by a lock-in
amplifier and the value of the Young's modulus (E) is calculated by
software as a function of the indentation depth d, using the
well-established Oliver and
Pharr method .
Ten indentation tests were performed on different sites of the film
characteristic curve of E as a function of depth was then computed
by averaging the
individual measurements. The Young's modulus (E) of the film was
derived as the
plateau value of the indentation modulus E = f(d) curve (Figure 5).
The estimated values
of Young modulus of the UNCD film were about 300-315 GPa, which are
those reported in the literature with values between 500 and 1000
GPa [13, 18, 20]. This
can be attributed to the presence of the grain boundary material.
Further tests with
various film thicknesses are needed in order to rule out the effect
of the substrate on our
measurements. Yet, this value is much higher than the Young's
modulus of Si.
Figure 5. The graph of recorded Young modulus as a function of
indentation depth into the film surface.
3.3. Stress estimation of UNCD films from analysis of FEM
calculations of fabricated microstructures
Series of double clamped beams of different lengths (in the range
300 - 510 µm)
were characterized by WLI (White Light Interferometry - FOGALE 3D).
show the first buckling mode (Figure 6), which means a compressive
existing in the UNCD film.
Figure 6. 3D WLI images of the bridge arrays; (a) the reconstructed
profiles of four constant-width groups
(widths of: 4.5, 6, 7.5, and 9 µm, respectively); (b) the
reconstructed profile of a constant-width group
which has bridges of increasing length (length range: 300 -510
For each of the bridges the buckling amplitudes, s, were measured
and tabulated in Table 1.
Table 1. Measured amplitudes (s) of the first buckling mode.
L [µm] 300 330 360 390 420 450 480 510
s [µm] 5.92 6.55 7.06 7.65 8.19 8.76 9.32 9.91
For guiding purposes, the assessment of the magnitude of the
residual stress from
buckling was initially considered with an analytical formula. The
stress is given analytically by the following expression [21,
2 2 2
πσ = +
where E is the Young's modulus of the material, t the beam's
thickness, s the out-of-
plane displacement amplitude of the first buckling mode, and L the
length of the beam.
Figure 7. A FEM simulated bridge (L=300 µm) that includes the bond
pads and the silicon pillars, showing the displacement in the first
buckling mode due to the compressive stress
However, the analytical model is an idealization of the
hence FEM (finite element method)-based simulations would be more
performed FEM calculations using COMSOL Multiphysics software to
find out the
value of the residual stress. In this case we assumed a uniform
stress in the plane of the UNCD layer, and a zero-gradient stress
along the thickness,
namely σxx(z) = σyy(z) = σ0. The FEM model was built using the
actual geometry of the
fabricated structures and the same material properties as used in
the analytical model. In
order to find the stress magnitude that creates the beams shapes, a
simulation was conducted, and the results were compared to the
measured values of
bucking mode amplitude for each simulated beam.
The dimensions of the microstructures and the material properties
simulations were those obtained from the design parameters and from
Thus, the thickness of the UNCD film, t, was set to 1 µm, and the
Young's modulus, E,
to 300 MPa, whilst the values of L and s were taken from Table 1. A
calculation of the bucking due the residual stress is presented in
Figure 7, where bond
pads and Si pillars were considered. In Figure 8 we show the
results of the film stress
calculated by both the analytical formula, Eq. (1), and by FEM
Figure 8. Analytical versus FEM calculations of stress values for
different beam lengths.
The analytical model gives an average value of the compressive
stress of about
290 MPa, while in the FEM calculations the value of stress is 350
MPa. The difference
between these two approaches is of approximately 20% but we must
bear in mind that
the FEM model was built to reproduce various details of the real
object. The FEM model
includes the bond pads of the bridges, the undercut, and the
silicon pillars. Thus, a series
of effects such as the non-ideal clamping (Figure 9) are not
considered in the ideal beam
model (the analytical approach) but are taken into account in the
FEM model. Also, in
the FEM analysis the geometric nonlinearities were considered,
contrary to the analytical
model where they are ignored. The value we have calculated for the
residual stress in the
UNCD film is within the bounds of the residual stress found in the
literature, where a
stress of a few hundreds of MPa can be encountered in UNCD films
[13, 18, 20].
Figure 9. Image showing the non-ideal clamping of the beam's end in
the FEM model. Displacements are exaggerated by a factor of 100 in
order to show the effect.
The buckling profiles obtained by WLI were used to check the
correctness of the
analytical and FEM models. The z-displacement of the beam within
the analytical model
of the first buckling mode is described by the following sinusoidal
function [21, 22]:
( ) 2 1
π = + , (2)
where x is the coordinate in the xy - plane of the beam. We must
notice here that only the
bucking amplitude s is involved in Eq. (2), but not the residual
stress. As it can be seen
from Figures 10 and 11, the analytical and FEM simulated shapes are
almost identical to
the WLI profile.
Figure 10. Comparison of WLI data, the FEM-based simulation, and
the analytical profile of the first buckling mode of a 300 µm long
Figure 11. WLI data against the FEM-based simulation and against
the analytical profile of the first buckling mode of a 500 µm long
In the present work we studied the fabrication of different
microstructures from UNCD films grown on Si substrate. The
fabrication was performed
without sacrificial layer by isotropic etching of the substrate.
Through a well-controlled
multi-step process, we fabricated arrays of bridges and cantilevers
dimensions. The bridges were buckled showing a residual stress
built in the UNCD film.
In order to estimate the residual stress, the Young's modulus was
measurements gave us a value of Young's modulus that ranges between
300 and 315
GPa. The knowledge of Young's modulus as well as the measurements
profiles by White Light Interferometry allowed the determination of
the residual stress
by finite element calculations performed with COMSOL software.
calculations provided us a stress value of 320 MPa, which is 20%
higher than the value
given by the analytical formula of an ideal beam model.
Acknowledgements. This research was supported by ANCSI, CORE -
Programme No. PN 16 32 02 01/2016: “Carbon nanostructures –
experimental and applicative investigations”.
 COE S. E., SUSSMANN R. S., Optical, thermal and mechanical
properties of CVD diamond, Diamond Relat. Mater., 9, pp. 1726−1729,
 HESS P., The mechanical properties of various chemical vapor
deposition diamond structures compared to the ideal single crystal,
J. Appl. Phys., 111, pp. 051101-9, 2012.
 LUO J. K., FU Y. Q., LE H. R., WILLIAMS J. A., SPEARING S. M.,
MILNE W. I., Diamond and diamond-like carbon MEMS, J. Micromech.
Microeng., 17, pp. S147-63, 2007.
 BERMAN D., KRIM J., Surface science, MEMS and NEMS: Progress
and opportunities for surface science research performed on, or by,
microdevices, Prog. Surf. Sci., 88, pp. 171-211, 2013.
 SHENDOROVA O. A., MCGUIRE G., Types of nanocrystalline diamond,
in O. A. Shenderova, D. M. Gruen, editors. Ultrananocrystalline
Diamond: Synthesis, Properties, and Applications, New York, NY:
William Andre, 2010.
 KULISCH W., POPOV C, SASAKI T., SIRGHI L., RAUCHER H., ROSSI
F., REITHMAIER J. P., On the development of themorphology of
ultrananocrystalline diamond films, Phys. Status Solidi A, 208, pp.
 KULISCH W., PETKOV C., PETKOV E., POPOV C., GIBSON P.N., VERES
M., MERZ R., MERZ B., REITHMAIER J.P., Low temperature growth of
nanocrystalline and ultrananocrystalline diamond films: A
comparison, Phys. Status Solidi A, 209, pp. 1664-1674, 2012.
 KRAUSS A.R., AUCIELLO O., GRUEN D.M., Ultrananocrystalline
diamond thin films for MEMS and moving mechanical assembly devices,
Diamond and Rel. Materials 10, pp. 1952- 1961, 2001
 MEHREGANY M., ZORMAN C.A., Surface micromachining: a brief
introduction, MRS Bull. 26, pp. 289-290, 2001.
 ALLEY R.L., MAI P., KOMVOPULOS K., HOWE R.T., Surface
roughness modification of interfacial contacts in polysilicon
microstructures, Proc. 7th Int. Conf. Solid-State Sensors and
Actuators-Transducers'93, Yokohama, Japan, pp. 288-292, 1993.
 ABE T., MESSNER W.C., REED M.L., Effects of elevated
temperature treatments in microstructure release procedures, J.
Microelectromech. Syst. 4, 66-75, 1995.
 MULHERN G.T., SOANE D.S., HOWE R.T., Supercritical carbon
dioxide drying of microstructures, Proc. 7th Int. Conf. Solid-State
Sensors and Actuators-Transducers'93, Yokohama, Japan, pp. 296-300,
 AUCIELLO O., BIRRELL J., CARLISLE J. A., GERBI J. E., XIAO X.,
PENG B., ESPINOSA H. D., Materials science and fabrication
processes for a new MEMS technology based on ultrananocrystalline
diamond thin films, J. Phys.: Condens. Matter, 16, pp. R539-R552,
 C. PACHIU, C. TIBEICA, A. AVRAM, M. VECA, T. SANDU, M.
POPESCU, R. POPA, " Processing and Mechanical Characterization of
Ultrananocrisytalline Diamond films for MEMS applications", IEEE
Proceedings CAS Conference, pp. 235-236, 2017.
 HAZARJARIBI Y., HAMIDON M. N., Reactive Ion Etching of 4H-SiC
Using SF6/O2 for MEMS Application, The International Journal Of
Engineering And Science, 2, pp. 87-92, 2013.
 PARK J. C., KIM S. H., KIM T. G., KIM J. K., CHO H., LEE B.
W., High density plasma etching of ultrananocrystalline diamond
films in O2/CF4 and O2/SF6 inductively coupled plasmas, Mod. Phys.
Lett. B, 29, pp. 1540022-5, 2015.
 AUCIELLO O., SUMANT A. V., Status review of the science and
technology of ultannocrystalline diamond (UNCDTM) films and
application to multifunctional devices, Diamond& Related
Materials, 19, pp. 699-718, 2010.
 OLIVER, W. C., PHARR, G. M., Measurement of hardness and
elastic modulus by instrumented indentation: advances in
understanding and refinements to methodology, J.Mater.Res.,19, pp.
 BUTLER J. E., SUMANT A. V., The CVD of Nanodiamond Materials,
Chem. Vap. Deposition, 14, pp. 145-160, 2008.
 LACONTE J., FLANDRE D., RASKIN J. -P., Micromachined Thin-Film
Sensors for SOI- CMOS Co-Integration, Springer, US, 2006.